Embed Size (px)
Transcript of Procedura Termosistem
Edition March 2000
Amendment June 2008
GUIDELINE FOR EUROPEAN TECHNICAL APPROVAL
EXTERNAL THERMAL INSULATION
COMPOSITE SYSTEMS WITH RENDERING
E O T A
Kunstlaan 40 Avenue des Arts B - 1040 BRUSSELS
European Organisation for Technical Approvals
Europische Organisation fr Technische Zulassungen
Organisation Europenne pour lAgrment Technique
ETAG 004 2
TABLE OF CONTENTS
Section one : INTRODUCTON
1 PRELIMINARIES 13
1.1 LEGAL BASIS 13
1.2 STATUS OF ETA-GUIDELINES 13
2 SCOPE 15
2.1 SCOPE 15
2.2 USE CATEGORIES, PRODUCTS FAMILIES, KITS AND SYSTEMS 15
2.3 ASSUMPTIONS 16
3 TERMINOLOGY 17
3.1 COMMON TERMINOLOGY AND ABBREVIATIONS 17
3.2 SPECIFIC TERMINOLOGY 17
3.2.1 Substrates 17
3.2.2 ETICS components 17
126.96.36.199 Adhesive 17
188.8.131.52 Insulation product 17
184.108.40.206 Rendering system 17
220.127.116.11 Mechanical fixing devices 18
18.104.22.168 Ancillary materials 18
3.2.3 ETICS description 18
22.214.171.124 Bonded ETICS 18
126.96.36.199 Mechanically fixed ETICS 18
Section two : GUIDANCE FOR THE ASSESSMENT OF THE FITNESS FOR USE
4 REQUIREMENTS 21
4.0 GENERAL 21
4.1 ER1 : MECHANICAL RESISTANCE AND STABILITY 23
4.2 ER2 : SAFETY IN CASE OF FIRE 23
4.3 ER3 : HYGIENE, HEALTH AND ENVIRONMENT 23
4.3.1 Indoor environment, dampness 23
4.3.2 Outdoor environment 24
4.3.3 Release of dangerous substances 24
4.4 ER4 : SAFETY IN USE 24
4.5 ER5 : PROTECTION AGAINST NOISE 26
4.6 ER6 : ENERGY ECONOMY AND HEAT RETENTION 26
4.7 ASPECTS OF DURABILITY AND SERVICEABILITY 26
5 METHODS OF VERIFICATION 28
ETAG 004 3
5.0 GENERAL 28
5.1 TEST ON THE ETICS 30
5.1.1 Mechanical resistance and stability 30
5.1.2 Safety in case of fire 30
188.8.131.52 Reaction to fire 30
5.1.3 Hygiene, health and the environment 31
184.108.40.206 Water absorption (capillarity test) 31
220.127.116.11 Watertightness 32
18.104.22.168.1 Hygrothermal behaviour 32
22.214.171.124.2 Freeze-thaw behaviour 36
126.96.36.199 Impact resistance 36
188.8.131.52.1 Resistance to hard body impact 37
184.108.40.206.2 Resistance to perforation (Perfotest) 37
220.127.116.11 Water vapour permeability (resistance to water vapour diffusion) 38
18.104.22.168 Release of dangerous substances 39
5.1.4 Safety in use 39
22.214.171.124 Bond strength 40
126.96.36.199.1 Bond strength between base coat and insulation product 40
188.8.131.52.2 Bond strength test between adhesive and substrate 41
184.108.40.206.3 Bond strength test between adhesive and insulation
220.127.116.11 Fixing strength (transverse displacement) 42
18.104.22.168.1 Displacement test 43
22.214.171.124 Wind load resistance of mechanically fixed ETICS 45
126.96.36.199.1 Pull-through tests of fixings 46
188.8.131.52.2 Static foam block test 47
184.108.40.206.3 Dynamic wind uplift test 49
5.1.5 Protection against noise 52
5.1.6 Energy economy and heat retention 52
220.127.116.11 Thermal resistance and thermal transmittance 52
5.1.7 Aspects of durability and serviceability 54
18.104.22.168 Bond strength after ageing 54
22.214.171.124.1 Finishing coat tested on the rig 54
126.96.36.199.2 Finishing coat not tested on the rig 54
TEST ON COMPONENTS 55
5.2 INSULATION PRODUCT 55
5.2.1 Mechanical resistance and stability 55
5.2.2 Safety in case of fire 55
5.2.3 Hygiene, health and the environment 55
188.8.131.52 Water absorption 55
184.108.40.206 Water vapour permeability 55
5.2.4 Safety in use 55
220.127.116.11 Tensile test perpendicular to the faces 55
18.104.22.168.1 In dry conditions 55
22.214.171.124.2 In wet conditions 55
126.96.36.199 Shear strength and shear modulus of elasticity test 56
ETAG 004 4
5.2.5 Protection against noise 56
5.2.6 Energy economy and heat retention 56
188.8.131.52 Thermal resistance 56
5.3 ANCHORS 56
5.3.1 Mechanical resistance and stability 56
5.3.2 Safety in case of fire 56
5.3.3 Hygiene, health and the environment 56
5.3.4 Safety in use 56
184.108.40.206 Pull-out strength of anchor 56
5.3.5 Protection against noise 57
5.3.6 Energy economy and heat retention 57
5.4 PROFILES AND THEIR FIXINGS 57
5.4.1 Mechanical resistance and stability 57
5.4.2 Safety in case of fire 57
5.4.3 Hygiene, health and the environment 57
5.4.4 Safety in use 57
220.127.116.11 Pull-through resistance of fixings from profiles 57
5.4.5 Protection against noise 58
5.4.6 Energy economy and heat retention 58
5.5 Render 58
5.5.1 Mechanical resistance and stability 58
5.5.2 Safety in case of fire 58
5.5.3 Hygiene, health and the environment 58
5.5.4 Safety in use 59
18.104.22.168 Render Strip Tensile Test 59
5.5.5 Protection against noise 61
5.5.6 Energy economy and heat retention 61
5.6 REINFORCEMENT 62
5.6.1 Mechanical resistance and stability 62
5.6.2 Safety in case of fire 62
5.6.3 Hygiene, health and the environment 62
5.6.4 Safety in use 62
5.6.5 Protection against noise 62
5.6.6 Energy economy and heat retention 62
5.6.7 Aspects of durability and serviceability 62
22.214.171.124 Glass fibre mesh Tearing strength and elongation of the
reinforcing fabric 62
126.96.36.199.1 Testing in the as-delivered state 63
188.8.131.52.2 Testing after ageing 63
184.108.40.206 Metal lath or mesh 63
220.127.116.11 Other reinforcements 63
6 ASSESSING AND JUDGING THE FITNESS FOR USE 64
6.0 GENERAL 64
6.1 ETICS 66
6.1.1 Mechanical resistance and stability 66
ETAG 004 5
6.1.2 Safety in case of fire 66
18.104.22.168 Reaction to fire 66
6.1.3 Hygiene, health and the environment 66
22.214.171.124 Water absorption (capillarity test) 66
126.96.36.199 Watertightness 66
188.8.131.52.1 Hygrothermal performance 66
184.108.40.206.2 Freeze-thaw performance 67
220.127.116.11 Impact resistance 67
18.104.22.168 Water vapour permeability 68
22.214.171.124 Release of dangerous substances 68
6.1.4 Safety in use 69
126.96.36.199 Bond strength 69
188.8.131.52.1 Bond strength between base coat and insulation product 69
184.108.40.206.2 Bond strength between adhesive and substrate 69
220.127.116.11.3 Bond strength between adhesive and insulation product 69
18.104.22.168 Fixing strength (transverse displacement) 70
22.214.171.124.1 Displacement test 70
126.96.36.199 Wind load resistance of mechanically fixed ETICS 70
188.8.131.52.1 Pull-through of fixings 70
184.108.40.206.2 Static foam block test 70
220.127.116.11.3 Dynamic wind uplift test 70
6.1.5 Protection against noise 70
6.1.6 Energy economy and heat retention 71
18.104.22.168 Thermal resistance 71
6.1.7 Aspects of durability and serviceability 71
22.214.171.124 Bond strength after ageing 71
TEST ON COMPONENTS 71
6.2 INSULATION PRODUCT 71
6.2.1 Mechanical resistance and stability 71
6.2.2 Safety in case of fire 71
6.2.3 Hygiene, health and the environment 71
126.96.36.199 Water absorption 71
188.8.131.52 Water vapour permeability 71
6.2.4 Safety in use 72
184.108.40.206 Tensile strength perpendicular to the faces 72
220.127.116.11 Shear strength and shear modulus of elasticity 72
6.2.5 Protection against noise 72
6.2.6 Energy economy and heat retention 72
18.104.22.168 Thermal resistance 72
6.3 ANCHORS 73
6.3.1 Mechanical resistance and stability 73
6.3.2 Safety in case of fire 73
6.3.3 Hygiene, health and the environment 73
6.3.4 Safety in use 73
22.214.171.124 Pull-out strength of anchor 73
ETAG 004 6
6.3.5 Protection against noise 73
6.3.6 Energy economy and heat retention 73
6.4 PROFILES AND THEIR FIXINGS 73
6.4.1 Mechanical resistance and stability 73
6.4.2 Safety in case of fire 73
6.4.3 Hygiene, health and the environment 73
6.4.4 Safety in use 73
126.96.36.199 Pull-through resistance of fixings from profiles 73
6.4.5 Protection against noise 73
6.4.6 Energy economy and heat retention 74
6.5 RENDER 74
6.5.1 Mechanical resistance and stability 74
6.5.2 Safety in case of fire 74
6.5.3 Hygiene, health and the environment 74
6.5.4 Safety in use 74
188.8.131.52 Render Strip Tensile Test 74
6.5.5 Protection against noise 74
6.5.6 Energy economy and heat retention 74
6.6 REINFORCEMENT 74
6.6.1 Mechanical resistance and stability 74
6.6.2 Safety in case of fire 74
6.6.3 Hygiene, health and the environment 74
6.6.4 Safety in use 74
6.6.5 Protection against noise 75
6.6.6 Energy economy and heat retention 75
6.6.7 Aspects of durability and serviceability 75
184.108.40.206 Glass fibre mesh Tearing strength and elongation of the reinforcing fabric 75
220.127.116.11 Metal lath or mesh 75
18.104.22.168 Other reinforcements 75
7 ASSUMPTIONS AND RECOMMENDATIONS UNDER WHICH THE FITNESS FOR
USE OF THE PRODUCT IS ASSESSED 76
7.0 GENERAL 76
7.1 DESIGN OF THE WORKS 76
7.2 PACKAGING TRANSPORT AND STORAGE 76
7.3 EXECUTION OF THE WORKS 76
7.3.1 Preparation of the substrate 76
22.214.171.124 Substrates suitable for bonded ETICS 76
126.96.36.199 Substrates suitable for mechanically fixed ETICS 77
7.3.2 Execution of the ETICS 77
7.4 MAINTENANCE AND REPAIR OF THE WORKS 77
Section three : ATTESTATION OF CONFORMITY
8 ATTESTATION AND EVALUATION OF CONFORMITY 78
ETAG 004 7
8.1 EC DECISIONS 78
8.2 TASKS AND RESPONSIBILITIES OF THE MANUFACTURER AND NOTIFIED BODIES 79
8.2.1 Tasks of the manufacturer 79
188.8.131.52 Factory production control 79
184.108.40.206 Testing of samples taken at the factory 79
220.127.116.11 Declaration of Conformity 79
8.2.2 Tasks of the manufacturer or the approved Notified Body 79
18.104.22.168 Initial Type Testing 79
8.2.3 Tasks of the approved Notified Body 80
22.214.171.124 Assessment of the factory production control system - initial
inspection and continuous surveillance 80
126.96.36.199 Certification 80
8.3 DOCUMENTATION 80
Section four : ETA CONTENT
9 THE ETA CONTENT 84
9.1 THE ETA CONTENT 84
Annexe A : COMMON TERMINOLOGY AND ABBREVIATIONS 85
A.1 Works and products 85
A.1.1 Construction works 85
A.1.2 Construction products 85
A.1.3 Incorporation 85
A.1.4 Intended use 85
A.1.5 Execution 85
A.1.6 System 85
A.2 Performances 85
A.2.1 Fitness for Intended use 86
A.2.2 Serviceability 86
A.2.3 Essential Requirements 86
A.2.4 Performance 86
A.2.5 Actions 87
A.2.6 Classes or levels 87
A.3 ETAG Format 87
A.3.1 Requirements 87
A.3.2 Methods of verification 87
A.3.3 Specifications 87
A.4 Working life 88
A.4.1 Working life (of works or parts of the works) 88
A.4.2 Working life (of products) 88
A.4.3 Economically reasonable working life 88
A.4.4 Maintenance 88
A.4.5 Normal maintenance 88
A.4.6 Durability 88
ETAG 004 8
A.5 Conformity 89
A.5.1 Attestation of conformity 89
A.5.2 Identification 89
A.6 Approval and Notified Body 89
A.6.1 Approval Body 89
A.6.2 Notified Body 89
A.7 Abbreviations 89
A.7.1 Abbreviations concerning the Construction products directive 89
A.7.2 Abbreviations concerning approval 90
A.7.3 General abbreviations 90
Annexe B : SYNOPSIS 91
Annexe C : METHODS RELATED TO THE IDENTIFICATION OF THE ETICS
C.1 Adhesives, base coats, key coats and finishing coats 92
C.1.1 Products as delivered 92
C.1.1.1 Density 92
C.1.1.2 Dry extract 92
C.188.8.131.52 Lime and polymer based products 92
C.184.108.40.206 Silicate based products 93
C.1.1.3 Ash content 93
C.1.1.4 Particle size grading 93
C.1.2 Fresh mortar 94
C.1.2.0 Preparation of mortar 94
C.220.127.116.11 Dry mortar 94
C.18.104.22.168 Paste requiring addition of cement and powder requiring
addition of extra binder 94
C.22.214.171.124 Ready to use paste 94
C.1.2.1 Water retention capability 94
C.1.2.2 Density of fresh mortar 96
C.1.3 Hardened base coat 96
C.1.3.1 Products with a thickness greater than 5 mm 96
C.126.96.36.199 Preparation and storing of test samples 96
C.188.8.131.52 Dynamic modulus of elasticity 96
C.184.108.40.206 Shrinkage test 98
C.1.3.2 Products with a thickness up to 5 mm : static modulus of elasticity,
tensile strength and elongation at break 98
C.2 Insulation product 98
C.2.1 Density measurement 98
C.2.2 Dimensional characteristics and appearance 99
C.2.2.1 Length and width 99
C.2.2.2 Thickness 99
C.2.2.3 Squareness 99
C.2.2.4 Flatness 99
C.2.2.5 Surface condition 99
C.2.3 Compression test 99
ETAG 004 9
C.2.4 Dimensional stability tests 99
C.3 Reinforcement 99
C.3.1 Mass per unit area 99
C.3.2 Ash content 99
C.3.3 Mesh size and number of filaments 100
C.3.4 Elongation 100
C.4 Mechanical fixing devices 100
C.4.1 Dimensions 100
C.4.2 Load characteristics if necessary 100
Annexe D : REACTION TO FIRE 101
1 General 101
2 Testing according to EN ISO 1182 102
2.1 Insulation product 102
2.2 Render coatings 102
2.2.1 Base coats and finishing coats 102
2.2.2 Key coats and decorative coats 102
2.3 Adhesive 102
2.4 Reinforcement 102
3 Testing according to EN ISO 1716 102
3.1 Insulation product 103
3.2 Render coating 103
3.3 Adhesive 103
3.4 Reinforcement 103
4 Testing according to EN 13823 103
4.1 Insulation product 104
4.2 Render coatings 105
4.3 Adhesive 105
4.4 Reinforcement 105
4.5 Application of test results 105
5 Testing according to EN ISO 11925-2 106
5.1 Insulation product 106
5.2 Render coatings 107
5.3 Adhesive 107
5.4 Reinforcement 107
5.5 Application of test results 107
Annexe E : ETA Model 109
ETAG 004 10
Background of the ETAG
This Guideline has been drawn up by the EOTA Working Group 04.04/11 - External Thermal
Insulation Composite Systems (ETICS).
The WG consisted of members from fourteen EU-countries (Austria, Belgium, Czech Republic,
Denmark, Finland, France (Convenor), Germany, Italy, Netherlands, Lithuania, Portugal, Slovak
Republic, Slovenia and the United Kingdom) and four European industrial organisations (EEWISA
(European External Wall Insulation Systems Association), EMO (European Mortars Organisation),
EUMEPS (European Manufacturers of Expanded Polystyrene) and EURIMA (European Insulation
The Guideline sets out the performance requirements for External Thermal Insulation Composite
Systems (ETICS) for the use as external insulation of building walls, the verification methods used to
examine the various aspects of performance, the assessment criteria used to judge the performance
for the intended use and the presumed conditions for the design and execution.
The UEAtc Directives for the Assessment of External Insulation Systems for Walls (Expanded
Polystyrene Insulation Faced with a Thin Rendering), June 1988 and UEAtc Technical Guide for the
Assessment of External Wall Insulation Systems Faced with Mineral Render, April 1992 have formed
part of the basis for the Guideline.
Reference documents are referred to within the body of the ETAG and are subject to the specific
conditions mentioned therein.
EOTA Guidance Document 004 The Provision of Data for Assessments Leading to ETA
COMMISSION DECISION 96/603/EC
ISO 7892: 1988 Vertical building elements - Impact resistance tests - Impact
bodies and general test procedures
EOTA ETAG 014 Plastic anchors for fixing of external thermal insulation composite
systems with rendering (short form: Plastic anchors for ETICS)
EN ISO 3386 1 and 2 Flexible cellular polymeric materials Determination of stress
strain characteristic in compression
Part 1 Low-density materials
Part 2 High-density materials
EN ISO 6946
EN ISO 6946/A1
Building components and building elements - Thermal resistance
and thermal transmittance - Calculation method
EN 12524 Building materials and products Hygrothermal properties -
Tabulated design values.
EN ISO 10211-1 Thermal bridges in building - Heat flows and surface temperatures
- Part 1: General calculation methods.
EN 1934 Thermal insulation - Determination of steady state thermal
transmission properties - Calibrated and guarded hot box
EN 1609 Thermal insulating products for building applications -
Determination of short term water absorption by partial immersion
ETAG 004 11
EN 12086 Thermal insulating products for building applications -
Determination of water vapour transmission properties
EN 1607 Thermal insulating products for building applications -
Determination of tensile strength perpendicular to the faces
EN 12090 Thermal insulating products for building applications -
Determination of shear behaviour
EN 196-1 Method of testing cement Determination of strength
EN 1602 Thermal insulating products for building applications -
Determination of the apparent density
EN 822 Thermal insulating products for building applications -
Determination of length and width
EN 823 Thermal insulating products for building applications -
Determination of thickness
EN 824 Thermal insulating products for building applications -
Determination of squareness
EN 825 Thermal insulating products for building applications -
Determination of flatness
EN 826 Thermal insulating products for building applications -
Determination of compression behaviour
Thermal insulating products for building applications -
Determination of dimension stability under constant normal
laboratory conditions (23C / 50% Relative Humidity).
Thermal insulating products for building applications -
Determination of dimensional stability under specified temperature
and humidity conditions
EN 13162 Thermal insulation products for buildings Factory made mineral
wool (MW) products - Specifications
EN 13163 Thermal insulation products for buildings Factory made products
of expanded polystyrene (EPS) - Specifications
EN 13164 Thermal insulation products for buildings Factory made products
of extruded polystyrene foam (XPS) - Specifications
EN 13165 Thermal insulation products for buildings Factory made rigid
polyurethane foam (PUR) products - Specifications
EN 13166 Thermal insulation products for buildings Factory made products
of fenolic foam (PF) - Specifications
EN 13501-1 (2002) Fire classification of construction products and building elements:
Part 1 Classification using test data from reaction to fire tests
EN ISO 1182 Reaction to fire tests for building products Non combustibility
EN 1716 Reaction to fire tests for building products Determination of the
heat of combustion
EN 11925 Reaction to fire tests for building products Ignitability when
subjected to direct impingement of flame
EC decision EC OJ (L 229 of 20/8/1997 Decision 97/556/EC as amended
EN ISO 1460 (1995) Metallic coatings Hot dip galvanized coatings on ferrous
ETAG 004 12
materials Gravimetric determination of the mass per unit area.
EN ISO 1461 (1999) Metallic coatings Hot dip galvanized coatings on fabricated iron
and steel articles Specifications and test methods
EN ISO 10244-2 Steel wire and wire products Non-ferrous metallic coatings on
steel wire- Part 2: Zinc or zinc alloy coatings
ASTM C91 Standard specification for masonry cement
EN ISO 13788 Hygrothermal performance of building components and building
elements - Internal surface temperature to avoid critical surface
humidity and interstitial condensation - Calculation methods
The edition of a reference document given in this list is that which has been adopted by EOTA for its
When a new edition becomes available, this supersedes the edition mentioned in the list only when
EOTA has verified or re-established (possibly with appropriate linkage) its compatibility with the
ETAG 004 13
S e c t i o n o n e : I N T R O D U C T I O N
1.1 LEGAL BASIS
This ETAG has been established in compliance with the provisions of the Council Directive
89/106/EEC (CPD) and has been established taking into account the following steps:
- issuing of the final mandate by the EC: 12 February 1997
- issuing of the final mandate by EFTA: 12 February 1997
- adoption of the Guideline 004- edition March 2000 by EOTA 13 October 1999
- endorsement of the Guideline 004- edition March 2000 by the EC / EFTA:
SCC opinion of 9-10 December 1999
EC letter of 11 August 2000
- adoption of the Guideline 004- edition by EOTA
- endorsement of the Guideline 004 edition by the EC / EFTA:
SCC opinion of
EC letter of
This document is published by the Member States in their official language or languages
according to Art 11/3 of the CPD.
This ETAG 004 edition supersedes the ETAG004 edition March 2000.
1.2 STATUS OF ETA-GUIDELINES
1.2.1 An ETA is one of two types of technical specifications in the sense of the EC 89/106
Construction Products Directive. This means that Member States shall presume that the
approved products are fit for their intended use, i.e. they enable works in which they are
employed to satisfy the Essential Requirements during an economically reasonable
working life, provided that:
- the works are properly designed and built,
- the conformity of the products with the ETA has been properly attested.
1.2.2 This ETAG is a basis for ETA's, i.e. a basis for technical assessment of the fitness for
use of a product for an intended use. An ETAG is not itself a technical specification in
the sense of the CPD.
This ETAG expresses the common understanding of the Approval Bodies, acting together within
EOTA, as to the provisions of the Construction Products Directive 89/106/EEC and of the
Interpretative Documents, in relation to the products and uses concerned, and is written within
the framework of a mandate given by the Commission and the EFTA secretariat, after
consulting the Standing Committee for Construction.
ETAG 004 14
1.2.3 When accepted by the European Commission after consultation with the Standing
Committee for Construction, this ETAG is binding for the issuing of ETA's for the
products for the defined intended uses.
The application and satisfaction of the provisions of an ETAG (examinations, tests and
evaluation methods) leads to an ETA and a presumption of fitness of a product for the defined
use only through an evaluation and approval process and decision, followed by the
corresponding attestation of conformity. This distinguishes an ETAG from a harmonized
European standard which is the direct basis for attestation of conformity.
Where appropriate, products which are outside of the precise scope of this ETAG may be
considered through the approval procedure without guidelines according to art. 9.2 of the CPD.
The requirements in this ETAG are set out in terms of objectives and of relevant actions to be
taken into account. It specifies values and characteristics, the conformity with which gives the
presumption that the requirements set out are satisfied, wherever the state of art permits and
after having been confirmed as appropriate for the particular product by the ETA.
ETAG 004 15
This guideline deals with "External Thermal Insulation Composite Systems (ETICS)" with
rendering intended for use as external thermal insulation to the walls of buildings. The walls are
generally made of masonry (bricks, blocks, stones ...) or concrete (cast on site or as
ETICS are designed and installed in accordance with the ETA-holder's design and installation
instructions. The ETICS comprise components which are factory-produced by the ETA-holder or
the component suppliers. The ETA-holder is ultimately responsible for the kit. all components of
the ETICS which should be specified by the ETA-holder.
The ETICS comprise prefabricated insulation product bonded onto the wall, or mechanically
fixed using anchors, profiles, special pieces, etc..., or a combination of adhesive and
mechanical fixings. The insulation product is faced with a rendering consisting of one or more
layers (site applied), one of which contains a reinforcement. The rendering is applied directly to
the insulating panels, without any air gap or disconnecting layer.
ETICS using other facings such as brick slips or tiles will be dealt with in subsequent parts.
ETICS where the connection between rendering and insulation product has no function in their
behaviour are not covered by this guideline.
The ETICS include special fittings (e.g. base profiles, corner profiles ...) to connect them to
adjacent building structures (apertures, corners, parapets ...).
The ETICS are designed to give the wall to which they are applied satisfactory thermal
insulation. They should provide a minimal thermal resistance in excess of 1 m.K/W. In special
use, smaller thicknesses of insulation can be used subject to checking that there is no particular
The ETICS can be used on new or existing (retrofit) vertical walls. They can also be used on
horizontal or inclined surfaces which are not exposed to precipitation.
The ETICS are non load-bearing construction elements. They do not contribute directly to the
stability of the wall on which they are installed. The ETICS can contribute to durability by
providing enhanced protection from the effects of weathering.
The ETICS are not intended to ensure the airtightness of the building structure.
2.2 USE CATEGORIES, PRODUCTS FAMILIES, KITS AND SYSTEMS
From the design point of view, ETICS are differentiated according to the methods of fixing:
1. Purely bonded ETICS
ETICS may be fully bonded (over the entire surface) or partially bonded in strips and/or dabs.
2. Bonded ETICS with supplementary mechanical fixings
The load is totally distributed by the bonding layer. The mechanical fixings are used primarily to
ETAG 004 16
provide stability until the adhesive has dried and act as a temporary connection to avoid the risk
of detachment. They can also provide stability in case of fire.
ETAG 004 17
Mechanically fixed ETICS:
3. Mechanically fixed ETICS with supplementary adhesive
The load is totally distributed by the mechanical fixings. The adhesive is used primarily to
ensure the flatness of the installed ETICS.
4. Purely mechanically fixed ETICS
The ETICS. are secured to the wall by mechanical fixings only.
Several categories have been adopted to correspond to the degree of exposure to impact in
use. These categories are defined in paragraph 220.127.116.11.
The provisions of this ETAG apply to the preparation and issue of European Technical Approvals in accordance with Art. 9.1 of the CPD and section 3.1 of the Common Procedural Rules.
The state of the art does not enable the development, within a reasonable time, of full and
detailed verification methods and corresponding technical criteria/guidance for acceptance for
some particular aspects or products. This ETAG contains assumptions taking account of the
state of art and makes provisions for appropriate, additional case by case approaches when
examining ETA-applications, within the general framework of the ETAG and under the CPD
consensus procedure between EOTA members.
The guidance remains valid for other cases which do not deviate significantly. The general
approach of the ETAG remains valid but the provisions then need to be used case by case in an
appropriate way. This use of the ETAG is the responsibility of the Approval Body which receives
the special application, and subject to consensus within EOTA.
In cases in which a certain provision of this ETAG is not or not fully applicable or a particular
aspect of a kit, kit component, assembled system and/or intended use to be assessed is not or
not sufficiently covered by the methods and criteria of the ETAG, the procedure of Art. 9.2 of the
CPD and section 3.2 of the Common Procedural Rules applies with regard to the deviation or
ETAG 004 18
3.1 COMMON TERMINOLOGY AND ABBREVIATIONS
(See Annex A)
For the meaning of these terms see EOTA document Common terms used in Guidelines for
European technical approval published on the EOTA website.
3.2 SPECIFIC TERMINOLOGY
The term "substrate" refers to a wall, which in itself already meets the necessary airtightness
and mechanical strength requirements (resistance to static and dynamic loads).
It may be faced with mineral or organic renders or paints or with tiles.
- Masonry walls:
Walls constructed from units of clay, concrete, calcium silicate, autoclaved aerated concrete or
stone laid using mortar and/or adhesive.
- Concrete walls:
Walls made of concrete either cast in situ or prefabricated at the factory.
3.2.2 ETICS components
The adhesive ( 18.104.22.168.), the base coat and the finishing coat ( 22.214.171.124.) can include a range
of binders from pure polymeric to pure cementitious. They are available in the following forms:
- Dry mortar, powder blended at the factory that requires only mixing with a quantity of water
specified by the manufacturer;
- Powder requiring addition of extra binder;
- Paste requiring addition of cement;
- Ready to use paste, supplied in workable consistency.
A product used for bonding the insulation product to the wall substrate.
126.96.36.199 Insulation product
A pre-fabricated product, with a high thermal resistance, which is intended to impart insulating
properties to the substrate to which it is applied.
Note: the insulation product is assessed by an own harmonized technical specification (ETA
acc. to ETAG or CUAP; hEN).
188.8.131.52 Rendering system
All the coats applied to the outer face of the insulation product together with the reinforcement.
Glass fibre mesh, metal lath or plastic mesh reinforcement (embedded) as well as fibres
(dispersed) in the base coat to improve its mechanical strength.
ETAG 004 19
For glass fibre mesh, differentiation is done between:
Standard mesh: embedded in the base coat all over the area and tied positively at
joints, mostly by overlapping,
Reinforced mesh: embedded in the base coat additionally to the standard mesh to
improve the impact rsistance, generally applied without overlapping.
- Render coating:
The rendering is applied to the insulation product in one or several coats (application of a
new coat on top of an existing dry coat).
Installation can also be done in several layers (putting one layer on top of a fresh layer).
Generally, multi-coat renders include the following:
Base coat: Coat applied directly onto the insulation product; the reinforcement is
embedded into it and provides most of the mechanical properties of the rendering,
Key coat: Very thin coat which may be applied to the base coat and is intended to
act as a preparation for the application of the finishing coat. It can also be eventually
used for aesthetic reason (for example in case of dark ribbed finishing coats),
Finishing coat: Coat which contributes to the protection against weathering and can
provide a decorative finish; it is applied onto the base coat with or without a key
Type of finishing coat: Where the only difference between two finishing coats is due
to the size of the aggregates, they are designed as one type.
Decorative coat: Coat which generally contributes to the aesthetic finishing (to cover
efflorescence ...) of finishing coat and can also provide supplementary protection
184.108.40.206 Mechanical fixing devices
Profiles, anchors, pins or any special fixing devices used to secure the ETICS to the substrate.
220.127.116.11 Ancillary materials
Any supplementary element, component or product used in the ETICS, e.g. to form joints
(mastics, corner strips, etc...) or to achieve continuity (mastic, joint-covers ...).
3.2.3 ETICS description
18.104.22.168 Bonded ETICS
ETICS where the connection to the substrate is ensured by bonding. They may or may not
include supplementary mechanical fixings.
22.214.171.124 Mechanically fixed ETICS
ETICS where the connection to the substrate is ensured by mechanical fixings. They may or
may not include supplementary bonding.
ETAG 004 20
S e c t i o n t w o : G U I D A N C E F O R T H E A S S E S S M E N T
O F T H E F I T N E S S F O R U S E
a) Applicability of the ETAG:
This ETAG provides guidance on the assessment of ETICS and their intended uses. It is the
manufacturer or producer who defines the ETICS for which he is seeking ETA and how it is to be
used in the works, and consequently the scale of the assessment.
b) General lay out of this section:
The assessment of the fitness of products with regard to their fitness for intended use in
construction works is a process with three main steps:
- Chapter 4 clarifies the specific requirements for the works relevant to the products and uses
concerned, beginning with the Essential Requirements for works (CPD art. 11.2) and then listing
the corresponding relevant characteristics of products,
- Chapter 5 extends the list in chapter 4 into more precise definitions and the methods available to
verify product characteristics and to indicate how the requirements and the relevant product
characteristics are described. This is done by test procedures, methods of calculation and of
- Chapter 6 provides guidance on the assessing and judging methods to confirm fitness for the
intended use of the ETICS,
- Chapter 7, assumptions and recommendations are only relevant in as far as they concern the
basis upon which the assessment of the ETICS is made concerning their fitness for the intended
c) Levels or classes or minimum requirements, related to the Essential Requirements and to the
product performance (see ID clause 1.2 and EC Guidance Paper E):
According to the CPD "Classes" in this ETAG refer only to mandatory levels or classes laid down,
in the EC-mandate.
This ETAG indicates however the compulsory way of expressing relevant performance
characteristics for the ETICS. If, for some uses at least one Member state has no regulations, a
manufacturer always has the right to opt out of one or more of them, in which case the ETA will
state "no performance determined" against that aspect, except for those properties for which, when
no determination has been made, the ETICS doesnt any longer fall under the scope of the ETAG;
such cases shall be indicated in the ETAG.
d) Working life (durability) and serviceability:
ETAG 004 21
The provisions, test and assessment methods in this guideline or referred to, have been written,
based upon the assumed working life of the ETICS for the intended use of at least 25 years,
provided that the ETICS is subject to appropriate use and maintenance (cf. chapter 7). These
provisions are based upon the current state of art and the available knowledge and experience.
An "assumed working life" means that it is expected that, when an assessment following the
ETAG-provisions is made, and when this working life has elapsed, the real working life may be, in
normal use conditions, considerably longer without major degradation affecting the Essential
Note: The real working life of a product incorporated in a specific works depends on the
environmental conditions to which that works is subject and the particular conditions of the design,
execution, use and maintenance of that works may be outside this ETAG. Therefore, it cannot be
excluded that in these cases the real working life of the product may also be shorter or loger than
the assumed working life.
The indications given as to the working life of an ETICS cannot be interpreted as a guarantee given
by the ETA-holder manufacturer or his representative or the Approval Body issuing the ETA. They
should only be regarded as a means for choosing the appropriate criteria for ETICS in relation to
the expected, economically reasonable working life of the works (based upon ID. 5.2.2).
e) Fitness for the intended use:
"Fitness for (the intended) use" of a construction product means that the product has such
characteristics that the works in which it is to be incorporated can, if properly designed and built,
1. satisfy the Essential Requirements when and where such works are subject to regulations containing such requirements (CPD Art. 2.1) and
2. be fit for their intended use, account being taken of economy, and in this connection satisfy the Essential Requirements for an economically reasonable working life, if normally maintained (see CPD Annex I, sentence 1 and 2).
In the case of kits, "fitness for (the intended) use" refers to:
a) the characteristics of the assembled system (they must be such that the works in which the kit is to be incorporated, assembled, applied or installed, can, if properly designed and built, satisfy the Essential Requirements when and where such works are subject to regulations containing such requirements), as well as
b) the characteristics of the components of the assembled system (they must be such that the assembled system, if properly assembled, has the characteristics referred to in clause a above).
ETAG 004 22
This chapter sets out the aspects of performance to be examined in order to satisfy the relevant
Essential Requirements, by:
- expressing in more detail, within the scope of the ETAG, the relevant Essential
Requirements of the CPD in the Interpretative Documents and in the mandate, for works or
parts of the works, taking into account the actions to be considered, as well as the expected
durability and serviceability of the works,
- applying them to the scope of the ETAG (product and where appropriate its constituents,
components and intended uses), and providing a list of relevant product characteristics and
other applicable properties. When a product characteristic or other applicable property is
specific to one of the Essential Requirements, it is dealt with in the appropriate place. If,
however, the characteristic or property is relevant to more than one Essential Requirement, it
is addressed under the most important one with cross reference to the other(s). This is
especially important where a manufacturer claims No performance determined for a
characteristic or property under one Essential Requirement and it is critical for the assessing
and judging under another Essential Requirement. Similarly, characteristics or properties
which have a bearing on durability may be dealt with under ER 1 to ER 6. Where there is a
characteristic which only relates to durability this is dealt with in 4.7.
This chapter also takes into account further requirements, if any (e.g. resulting from other EC
Directives) and identifies aspects of serviceability including specifying characteristics needed to
identify the products (cf. ETA-format II.2).
The following Table 1 presents an overview of the Essential Requirements, the relevant
paragraphs of the corresponding Interpretative Documents and the related requirements to
ETAG 004 23
Table 1. Relationship between ID paragraph for works, ID paragraph for product
performance, product characteristic given in the mandate and ETAG paragraph on
ID paragraph for
1 - - - -
Limitation of spread of
fire and smoke beyond
the room of origin:
Limitation of spread of
fire to neighbouring
External walls and
Reaction to fire
Facades / external walls
- fire propagation
Reaction to fire (for
application of ETICS
subject to fire
Reaction to fire
Walls, walling materials
Impact resistance: hard
body impact and per-
4.3.3 Release of
Impacts of falling
objects, forming part of
the works, upon users
Fixing strength (for
Bond strength (for
Movements of the
5 - - - -
Thermal resistance 4.6
ETAG 004 24
ability - ... shrinkage
4.1 ER1: MECHANICAL RESISTANCE AND STABILITY
Requirements with respect to the mechanical resistance and stability of non load bearing parts
of the works are not included in this Essential Requirement but are treated under the Essential
Requirement Safety in use (see Clause 4.4).
4.2 ER2: SAFETY IN CASE OF FIRE
The Essential Requirement laid down in the council Directive 89/106/EEC is as follows: The
construction works must be designed and built in such a way that in the event of an outbreak of
- the load bearing capacity of the construction can be assumed for a specific period of time,
- the generation and spread of fire and smoke within the works are limited,
- the spread of fire to neighbouring construction works is limited,
- occupants can leave the works or be secured by other means,
- the safety of rescue teams is taken into consideration.
The following aspects of performance are relevant to this Essential Requirement for ETICS:
Reaction to fire:
The reaction to fire performance of ETICS shall be in accordance with laws, regulations and
administrative provisions applicable to the ETICS in its intended end use application. This
performance shall be expressed in the form of a classification specified in accordance with the
relevant EC decision and the relevant CEN classification standards.
4.3 ER3: HYGIENE, HEALTH AND ENVIRONMENT
4.3.1 Indoor environment, dampness
As far as dampness is concerned for external walls, two requirements have to be considered,
for which ETICS have a favourable effect:
- moisture proofing from outside damp
Walls should prevent moisture from the ground from entering the building and should not
carry moisture from the ground to any part where it could cause damage.
External walls should also resist the penetration of rain and snow to the inside of the
building; they should not be damaged by rain and snow and should not carry moisture to any
part where it could cause damage.
- avoiding condensation on internal surfaces and interstitial condensation. Surface
condensation is usually reduced by the application of ETICS.
Under normal conditions of use, harmful interstitial condensation does not occur in the ETICS.
Where there is a high incidence of water vapour internally, appropriate precautions must be
ETAG 004 25
taken to prevent the ETICS from becoming damp, for example by suitable design of the
products and choice of materials.
To ensure that the first of the above mentioned characteristics is sufficiently retained, the
performance on exposure to mechanical stresses under normal use should be considered, i.e.:
- the ETICS shall be designed so that it retains its properties under the effect of impacts
caused by normal traffic and normal use. Its performance should be such that the effect of
normal accidental or deliberately caused unexceptional impact does not cause any damage,
- it should be possible to lean standard maintenance equipment against the ETICS, without
causing any breaks or perforation of the render.
This means that for ER3 the following product characteristics have to be assessed for the
ETICS and/or each of its components:
- water absorption,
- impact resistance,
- water vapour permeability,
- thermal characteristics (covered under ER6).
4.3.2 Outdoor environment
Installation and construction works shall not release pollutants to the immediate environment
(air, soil, water).
The rate of release of pollutants to outdoor air, soil and water for building materials used in
external walls shall therefore be in accordance with laws, regulations and administrative
provisions, applicable for the location where the product is incorporated in the works.
4.3.3 Release of dangerous substances
The product/kit must be such that, when installed according to the appropriate provisions of the
Member States, it allows for the satisfaction of the ER3 of the CPD as expressed by the national
provisions of the Member States and in particular does not cause harmful emission of toxic
gases, dangerous particles or radiation to the indoor environment nor contamination of the
outdoor environment (air, soil or water).
4.4 ER4: SAFETY IN USE
Even though ETICS is without a structural intended use, mechanical resistance and stability is
The ETICS shall be stable to the combined stresses generated by normal loads such as intrinsic
weight, temperature, humidity and shrinkage, as well as movements of the main structure and
wind forces (suction).
This means that for ER 4 ETICS, the following products characteristics have to be assessed for
the ETICS and/or its components.
Effect of intrinsic weight:
ETAG 004 26
The ETICS shall support itself without harmful deformation.
Performance on exposure to movements of the main structure:
Normal movements of the main structure shall not give rise to any crack formation or loss of
adhesion in the ETICS. It is considered that the ETICS should withstand movements due to the
temperature and stress variations except at structural joints where special precautions have to be
ETAG 004 27
Effect of the wind suction:
The ETICS shall, with a sufficient safety factor, exhibit appropriate mechanical resistance to the
forces of pressure, suction and vibration, due to wind.
4.5 ER5: PROTECTION AGAINST NOISE
Requirements with respect to the protection against noise are not addressed, since these
requirements should be satisfied by the entire wall including the ETICS as well as windows and
4.6 ER6: ENERGY ECONOMY AND HEAT RETENTION
The entire wall should satisfy this requirement.
ETICS improve thermal insulation and make it possible to reduce heating (in winter) and air
conditioning (in summer).
Therefore the improvement of the thermal resistance of the wall introduced by the ETICS shall
be assessed so that it can be introduced in the thermal calculations required by the national
regulations on energy consumption.
Mechanical fixings or temporary anchor fixings can cause localised differences in temperature.
Assurance must be obtained that this effect is small enough not to influence the thermal
In order to establish the benefits of the ETICS to the wall, relevant component characteristics
shall be specified as follows:
- thermal conductivity/resistance,
- water vapour permeability (covered under ER3),
- water absorption (covered under ER3).
4.7. ASPECTS OF DURABILITY AND SERVICEABILITY
All of the ERs mentioned above must be fulfilled for the life of the ETICS under the actions to
which it is subjected.
Comment: It should be noted that the substrate can influence the ETICS durability.
Durability of the ETICS:
The ETICS shall be stable to temperature, humidity and shrinkage.
Neither high nor low temperatures shall exercise a destructive or irreversibly deforming effect.
Low air temperatures of the order of - 20C and high air temperatures of + 50C are generally
regarded as the extremes in temperature change. In northern European countries however, the
temperatures of the air can decrease to - 40C.
Solar radiation increases the surface temperatures of the ETICS when exposed. The increase
depends on the radiation flow and the energy absorption of the surface (colour). It is generally
considered that the maximum surface temperature is 80C.
A change (of the order of 30C) in the surface temperature shall not cause any damage, eg a
sudden change due to prolonged exposure to solar radiation followed by intensive rain, or the
change of temperature between sun and shade.
ETAG 004 28
In addition, steps shall be taken to prevent crack formation both at the expansion joints of the
structure and where elements of the facade are of different materials, e.g. connections to
Durability of components
All components shall retain their properties during the overall service life of the ETICS under
normal conditions of use and maintenance such that the ETICS quality is maintained. This
requires the following:
- All components shall display a chemical-physical stability and be at least reasonably
predictable if not absolutely known. Where reactions between materials in contact occur they
should take place slowly,
- All materials shall be either naturally resistant to, or be treated or protected against attack by
- All materials shall be compatible with each other.
ETAG 004 29
5 METHODS OF VERIFICATION
This chapter refers to the verification methods used to determine the various aspects of
performance of the products in relation to the requirements for the works (calculations, tests,
engineering knowledge, site experience, etc).
In order to assess and judge ETICS it is often necessary to adopt verification methods which
require the testing of two or more components in a small scale assembly. As such, they are
neither ETICS nor components. By taking this approach, it is possible to either avoid a large
number of full scale tests or at least limit the number required, by enabling the selection of the
appropriate combination of components to provide an assessment of the complete range.
Therefore, the structure of this chapter is that these tests relate to the system rather than to the
The relevant Essential Requirements, the relevant verification methods and the related product
characteristics to be assessed are indicated in the following table (Table 2).
Table 2. Relationship between ETAG paragraph on product performance, product
characteristic and ETAG paragraph on verification method for the ETICS or component.
ER ETAG Paragraph on product performance
Product characteristic ETAG paragraph on verification method
1 - - - -
2 4.2 Reaction to fire
Reaction to fire
5.1.2 ETICS 126.96.36.199 Reaction to fire
5.2 INSULATION PRODUCT 5.2.2 Reaction to fire
3 4.3 Water absorption Watertightness Impact resistance Water vapour permeability Outdoor environment
Water absorption Watertightness Impact resistance Water vapour permeability Release of dangerous substances
5.1.3 ETICS 188.8.131.52 Water absorption (capillarity test)
184.108.40.206.1 Hygrothermal behaviour 220.127.116.11.2 Freeze/thaw behaviour
18.104.22.168 Impact resistance
22.214.171.124.1 Resistance to hard body impact 126.96.36.199.2 Resistance to perforation
188.8.131.52 Water vapour permeability
184.108.40.206 Release of dangerous substances
5.2.3 INSULATION PRODUCT 220.127.116.11 Water absorption 18.104.22.168
Water vapour permeability
ETAG 004 30
Bond strength Fixing strength (transverse displacement) Resistance to wind load
5.1.4 ETICS 22.214.171.124 Bond strength
126.96.36.199.1 Bond strength between base coat and insulation product 188.8.131.52.2 Bond strength between adhesive and substrate 184.108.40.206.3 Bond strength between adhesive and insulation product
220.127.116.11 Fixing strength (transverse displacement)
18.104.22.168.1 Displacement test
22.214.171.124 Wind load resistance
126.96.36.199.1 Pull-through tests of fixings 188.8.131.52.2 Static foam block test 184.108.40.206.3 Dynamic wind uplift test
5.2.4 INSULATION PRODUCT 220.127.116.11 Tensile strength perpendicular to the faces 18.104.22.168 Shear strength and shear modulus of elasticity
5.3.4 ANCHORS 22.214.171.124 Pull-out strength of anchors
5.4.4 PROFILES 126.96.36.199 Pull-through resistance of fixings from profiles
4 4.4 Intrinsic weight Movements of the main structure Resistance to wind load
5.5.4 RENDER 188.8.131.52 Render strip tensile test
5 - - - -
6 4.6 Thermal resistance
5.1.6 ETICS 184.108.40.206 Thermal resistance
5.2.6 INSULATION PRODUCT 220.127.116.11 Thermal resistance
Aspects of durability and serviceability
4.7 Resistance to temperature, humidity and shrinkage
5.1.7 ETICS Resistance to temperature, humidity and shrinkage Resistance to freeze/thaw Dimensional stability (treated under relevant ERs) 18.104.22.168 Bond strength after ageing
5.6.7 REINFORCEMENT 22.214.171.124 Glass fibre mesh Tearing strength and elongation 126.96.36.199 Metal lath or mesh 188.8.131.52 Other reinforcements
ETAG 004 31
The tests described in the following may not all be necessary if the product is not new and has
been used for several years, so that existing data are available, see EOTA Guidance Document
no.004 on The Provision of Data for Assessments Leading to ETA (TB 98/31/12.6).
Until December 2008, instead of using the method described in 184.108.40.206.1, the performance with
regard to the characteristic concerned may also be established by long term experience on site,
provided that satisfactory technical argument is given in the Evaluation Report on the following
- this long term experience is well documented concerning particularly evidence of full
tracability back to the product originally installed,
- the ETICS subject to the approval procedure is the same as the ETICS for which the
performance is established by long term experience.
5.1 TEST ON THE ETICS
As much as possible (all tests carried out at the same time for example), all the tests shall be
performed on the same production lot for each component.
5.1.1 Mechanical resistance and stability
5.1.2 Safety in case of fire
220.127.116.11 Reaction to fire
The ETICS shall be tested, using the test method(s) relevant for the corresponding reaction to
fire class, in order to be classified according to EN 13501-1: 2002.
If no performance is determined, the products fall in class F without testing.
Method of the test:
The determination of the worst case(s) as well as the mounting and fixing provisions that are
considered to be appropriate for the testing and are representative of the intended end use
application are specified in Annex D.
Note: An European reference fire scenario has not been laid down for faades. In some
Member States, the classification of ETICS according to EN 13501-1:2002 might not be
sufficient for the use in faades. An additional assessment of ETICS according to national
provisions (e.g. on the basis of a large scale test) might be necessary to comply with Member
State regulations, until the existing European classification system has been completed.
ETAG 004 32
5.1.3 Hygiene, health and the environment
18.104.22.168 Water absorption (capillarity test)
These tests have 3 purposes, to determine:
- the water absorption, in order to assess, in Chapter 6, whether it is acceptable,
- which finishing coats should be applied on the rig to be subjected to hygrothermal testing
- whether the freeze-thaw testing described in 22.214.171.124.2 is necessary.
Preparation of the samples:
Samples are prepared, each by taking a piece of the specified insulation product, surface area
to be at least 200 mm x 200 mm, and applying, in accordance with the ETA-applicants
instructions, e.g. thickness, mass per unit area and method of application, both:
- the reinforced base coat alone
- all the configurations of complete rendering systems proposed by the ETA-holder, i.e.
reinforced base coat covered with each type of finishing coat associating or not key coat
and/or decorative coat. If the application of the key coat and/or the decorative coat is
optional, at least configurations without them shall be tested.
Exception for not testing all the above mentioned configurations can be accepted provided that
a technical argumentation is given in the Evaluation Report.
Within a type of finishing coat, the test shall be carried out with at least the higher layer
(generally higher particles size grading with floated finishing aspect).
Three samples are prepared for each configuration. Quantities and/or thicknesses applied
shall be recorded as well as identification of the renders components according to Annex C.
The prepared samples are conditioned for at least 7 days at (23 2)C and (50 5) % RH.
The edges of the samples, including the insulation product, are sealed against water, to
ensure that during subsequent testing, only the face of the reinforced base coat or the
rendering system is subject to water absorption.
They are then subject to a series of 3 cycles comprising the following phases:
- 24 h immersion in a water bath (tap water) at (23 2)C. The samples are immersed
rendered face downwards, to a depth of 2 to 10 mm, the depth of immersion dependent
upon surface roughness. To achieve complete wetting of rough surface, the samples shall
be tilted as they are introduced into the water. The depth of immersion can be regulated in
the water tank by means of a height-adjustable slat.
- 24 h drying at (50 5)C.
If interruptions are necessary, e.g. at week-ends or holidays, the samples are stored at
(23 2)C and (50 5)% RH after the drying at (50 5)C.
After the cycles, the samples are stored at least for 24 h at (23 2)C and (50 5)% RH.
Capillarity test procedure:
ETAG 004 33
To start the capillarity test the samples are again immersed in a water bath as described
The samples are weighed after 3 minutes immersion in the bath (reference weight) and then
after 1 hour and 24 hours. Prior to the second and subsequent weighing, water adhering to the
surface of the sample is removed with a damp sponge cloth.
Analysis of results:
Calculation is undertaken to determine the mean water absorption of the three samples per
square metre after 1 and 24 hours. The outcome of these results will determine the following:
- Acceptability of the ETICS : see 126.96.36.199
- Hygrothermal behaviour :
For the choice of the finishing coats to be applied on the rig, see Annex B and 188.8.131.52.1
- Freeze/Thaw test: see Annex B
The freeze/thaw test ( 184.108.40.206.2.) is necessary if the water absorption of either the
reinforced base coat or of the rendering coating is equal to or more than 0.5 kg/m after 24
Footnote Special requirements for some ETICS:
- In order to provide information about the stabilisation, the water absorption measured can be
plotted on a chart as a function of t ,
- If the ETICS is applied down to the ground and is therefore exposed to rising damp, the
Approval Body may need to develop additional tests in an appropriate way subject to
consensus within EOTA.
220.127.116.11.1 Hygrothermal Behaviour
Based on the outcome of the water absorption test, the specification to be tested is
determined, e.g. the number of finishing coats (see Annex B)
Some samples are prepared at the same time as the rig in order to evaluate the following
characteristics after heat/rain and heat/cold cycles (for sample size and number: see
relevant test method):
- Bond strength between the base coat and insulation product (only if the low part of the rig
does not only consist of the reinforced base coat alone, i.e. ETICS with only one finishing
- Tensile strength and elongation at break (Annex C, C1.3.2) (for products with an
application thickness up to 5 mm).
In case of reinforced base coat with a thickness greater than 5 mm, complementary samples
shall also be prepared to perform the test on hardened product according to Annex C
Principles related to the preparation of the rig:
- As a general rule, only one reinforced base coat and at the very most four finishing coats
(vertical divisions) can be applied per rig.
ETAG 004 34
- If several adhesives are proposed for the ETICS, only one shall be tested on the rig.
Further testing is described in 18.104.22.168.
- If more than 4 finishing coats are proposed for the ETICS, the maximum number of coats,
representative of the different types proposed, shall be tested on rig(s). Furthermore, if
the water absorption of the reinforced base coat after 24 h is equal to or more than 0.5
kg/m (see 22.214.171.124), each type of finishing coat containing a pure polymeric binder (non
cementitious) shall be submitted to hygrothermal cycles on rig(s) . Any finishing coats not
tested on the rig shall be examined according to 126.96.36.199.2.
Note: Where the only difference between two finishing coats is due to the size of
aggregates, they are designated as one type.
- If different finishing coats can be used in the ETICS, the lower part of the test piece (1,5 x
insulating panel height) consists of the reinforced base coat only without any finishing
- If several ETICS differ only in the method of fixing (bonded or mechanically fixed) of the
insulation product, the test is only carried out on the ETICS applied with adhesive at the
edge of the rig and with mechanical fixings devices in the centre.
- If several ETICS differ only in the type of insulation product, two can be applied to the rig.
The insulation products are divided vertically at the centre of each rig.
- The ETICS is applied, in accordance with the manufacturers instructions, to a sufficiently
stabilised masonry or concrete substrate.
- The ETICS should also be applied to the lateral faces with a uniform maximum thickness
of insulation product of 20 mm. If the insulation product is not available in this thickness
(Mineral wool Lamella for example), the lateral faces can be covered with a thickness of
20 mm expanded polystyrene.
- Insulation product requiring stabilisation (prescribed delay between production and sale)
shall be no older than 15 days beyond the minimum specified period.
- The dimensions of the rig shall be:
- - surface > 6 m
- - width > 2.50 m
- - height > 2.00 m
An opening (consisting in an absence of the ETICS on the substrate at this area) is included
at the corner of the rig, 0.40 m wide by 0.60 m high, positioned 0.40 m from the edges.
ETAG 004 35
Fig. 1. Dimensions of the rig (quoted in metres)
Remark: if two insulation products are foreseen to be applied to the rig, two symmetrical
openings shall be included at both of the upper corners of the rig.
Special methods for reinforcing corners of the opening are applied, if necessary.
Installation of the window sill is the responsibility of the ETA applicant.
Preparation of the rig:
The rig preparation shall be made by an applicant designated by the ETA-holder. It shall be
supervised by the third laboratory in charge of the test regarding:
- in case of insulation product requiring stabilisation (prescribed delay between production
and sale), verification that it is not older than 15 days beyond the minimum specified
- checking of the respect of manufacturer prescriptions : all stages shall be in accordance
with the Technical File of the ETA-holder
- registering of all the stages of the installation :
- the date and time of the various stages
- temperature and % Relative Humidity during the installation (every day at least at
- name and production lot of the components
- way of fixing the insulation product
- figure describing the rig (place of the fixings and of the joints between the panels, )
- way of renders preparation (tool, % of mixing, possible pause time before application,
) as well as their way of application (hand tool, machines, number of layers,)
- quantities and/or thickness of renders applied per square metre
- drying period between each layer
- use and position of accessories
- any other information
Quantities and/or thicknesses applied shall be recorded as well as identification of the
renders components according to Annex C.
Conditioning of the rig:
The ETICS is cured inside for a minimum of 4 weeks. During the curing time the ambient
temperature shall be between 10C and 25C. The relative humidity shall not be less than
50 %. To ensure that these conditions are met, records shall be made at regular intervals. To
ETAG 004 36
prevent the ETICS from drying out too rapidly the ETA applicant may require the render to
be wetted once per week by spraying for approximately 5 minutes. This should start
according to the prescriptions of the ETA-holder.
During the curing time any deformations of the ETICS, i.e. blistering, cracking, are recorded.
For a reinforced base coat with a thickness up to 5 mm, some samples are prepared
according to Annex C C.1.3.2 and placed in the opening of the rig.
The test apparatus is positioned against the front face of the rig, 0.10 to 0.30 m from the
The specified temperatures during the cycles are measured at the surface of the rig. The
regulation shall be obtained by adjustment of the air temperature.
Heat - rain cycles:
The rig is subjected to a series of 80 cycles, comprising the following phases:
1- heating to 70C (rise for 1 hour) and maintaining at (70 + 5)C and 10 to 30% RH for
2 hours (total of 3 hours),
2- spraying for 1 hour (water temperature (+ 15 5)C, amount of water 1 l/m min),
3- leave for 2 hours (drainage).
After at least 48 hours of subsequent conditioning at temperatures between 10 and 25C and
a minimum relative humidity of 50 %, the same test rig is exposed to 5 heat/cold cycles of
24 hours comprising the following phases:
1- exposure to (50 5)C (rise for 1 hour) and maximum 30% RH for 7 hours (total of
2- exposure to (- 20 5)C (fall for 2 hours) for 14 hours (total of 16 hours).
Observations during the test:
At periods of every four cycles during the heat/rain cycles and at every cycle during the
heat/cold cycles, observations relating to a change in characteristics or performance
(blistering, detachment, crazing, loss of adhesion, formation of cracks, etc ...) of the entire
ETICS and of the part of the rig consisting of only the reinforced base coat are recorded as
- the surface finish of the ETICS is examined to establish whether any cracking has
occurred. The dimensions and position of any cracks should be measured and recorded,
- the surface should also be checked for any blistering or peeling and the location and
extent should again be recorded,
- the sills and profiles should be checked for any damage/degradation together with any
associated cracking of the finish. Again, the location and extent should be recorded.
Following the completion of the test, a further investigation is conducted involving removal of
sections containing cracks to observe any water penetration within the ETICS.
After the heat-rain and heat-cold cycles
ETAG 004 37
Bond strength tests according to 188.8.131.52.1 and 184.108.40.206.1. and impact resistance test
according to 220.127.116.11 shall be performed, after at least 7 days drying.
ETAG 004 38
18.104.22.168.2 Freeze-thaw behaviour
The freeze-thaw test shall be carried out as determined by the analysis of the capillarity test
( 22.214.171.124), i.e. shall be conducted except if the water absorption after 24 hours of both the
reinforced base coat and the rendering system determined with each type of finishing coat is
less than 0.5 kg/m.
The test shall be carried out on three samples 500 mm x 500 mm consisting of a piece of the
specified insulation product covered by:
- reinforced base coat without finishing coat if its water absorption is equal or higher
than 0.5 kg/m,
- all the configurations of rendering systems proposed by the ETA-holder (i.e.
reinforced base coat covered with each type of finishing coat associating or not key
coat and/or decorative coat which lead to a water absorption equal or higher than
0.5 kg/m. If the application of the key coat and/or the decorative coat is optional, at
least configurations without them shall be tested).
These samples are prepared according to the ETA applicants instructions and then stored
for at least 28 days at (23 + 2)C and (50 + 5) % RH.
Quantities and/or thicknesses applied shall be recorded as well as identification of the
renders components according to Annex C.
The samples are then subjected to a series of 30 cycles comprising:
- Exposure to water for 8 hours at initial temperature of (23 2)C by immersion of
the samples, render face downwards, in a water bath, by the method described in
126.96.36.199 Capillarity test,
- Freezing to (- 20 2)C (fall for 5 hours at the sample surface and for 2 hours in
the conditioned air) for respectively 11 and 14 hours (total of 16 hours).
If the test is interrupted, because the samples are handled manually and there are stops
during weekends or holidays, the samples shall always be maintained in immersion in water
between the cycles.
Remark: The specified temperatures are measured at the surface of the samples. The
regulation is obtained by conditioned air.
At the end of the test, observations relating to a change in characteristics of the surface or to
the behaviour of the entire ETICS are recorded according to 188.8.131.52.1.
Any distortion at the edges of the samples shall also be reported.
After the test
A bond strength test shall be performed in accordance with 184.108.40.206.1 on each sample
submitted to freeze-thaw cycles.
220.127.116.11 Impact resistance
ETAG 004 39
These tests are performed on the rig after the heat-rain and the heat-cold cycles.
For finishing coats not tested on the rig or for complementary tests (double meshes, etc),
these tests can also be carried out on samples aged by immersion in water for 6 to 8 days
and then dried for at least 7 days at (23 2)C and (50 5)% RH. Within a type of finishing
coat, the test shall be carried out with at least the lower layer (generally lower particles size
grading with ribbed finishing aspect). Quantities and/or thicknesses applied shall be recorded
as well as identification of the renders components according to Annex C.
In case of test with reinforced mesh, the extrapolation of results to very different products
(other mesh size, other mass per unit area, etc) shall be carefully examined.
In case of possible optional use of key coat and/or decorative coat, at least the configurations
without them shall be tested.
18.104.22.168.1 Resistance to hard body impact
Hard body impact tests are performed as described in ISO 7892: 1988, "Vertical building
elements - Impact resistance tests - Impact bodies and general test procedures". The points of
impact are selected taking into account various modes of behaviour of walls and their
cladding, varying according to whether the impact point is or is not located in an area of
greater rigidity (reinforcement).
Hard body impacts (10 Joules) are carried out on 3 samples with the steel ball weighing 1 kg
and from a height of 1.02 m
Hard body impacts (3 Joules) are carried out on 3 samples with the steel ball weighing 0.500
kg and from a height of 0.61 m.
- the diameter of the impact is measured and indicated,
- the presence of any micro cracks or cracks, at the impact point and at the circumference, is
22.214.171.124.2 Resistance to perforation (Perfotest)
Where the thickness of the reinforced base coat is less than 6 mm, "Perfotest" shall be
carried out in addition.
"Perfotest" (Fig. 2) is an apparatus which enables perforating impacts to be reproduced. It is
calibrated with a hemispherical indentor (Fig. 3) reproducing the impact of a steel sphere
weighing 0.500 kg falling from 0.765 m.
The measurements are taken on 5 samples with the perforating cylindrical indentors shown
in the following pictures.
The diameter of the indentor used without perforating the rendering is to be noted.
ETAG 004 40
Fig. 2: Perfotest apparatus
Cylindrical indentor Hemispherical indentor (for calibration)
No 1 2 3 4 5 6 7 8 9
D A B
4 10 20
6 10 20
8 15 15
10 15 15
12 15 15
15 15 15
20 15 15
25 15 15
30 15 15
Dimensions in mm
Quenched and tempered steel (R= 180 kgmm-2
Fig. 3: Indentors
126.96.36.199 Water vapour permeability (resistance to water vapour diffusion)
The test shall be performed on all the configurations of rendering systems proposed by the
ETA-holder, i.e. reinforced base coat covered with each type of finishing coat associating or
not key coat and/or decorative coat. If the application of the key coat and/or the decorative
coat is optional, configurations with and without shall be tested.
ETAG 004 41
Within a type, the test shall be carried out with the thickest continuous layer (generally higher
particles size grading with floated finishing aspect).
Exception for not testing all the above mentioned configurations can be accepted provided that
a technical argumentation is given in the Evaluation Report.
The samples are prepared by applying the rendering to the insulation product in accordance
with the ETA applicants instructions and conditioned for at least 28 days at
(23 + 2)C and (50 + 5)% RH. Quantities and/or thicknesses applied shall be recorded as well
as identification of the renders components according to Annex C.
Five test samples of at least 5000 mm are then obtained by separating the rendering system
from the insulation product.
The test is carried out in accordance with EN 12086, Thermal insulating products for buildings
application - Determination of water vapour transmission properties.
The test should be carried out in an enclosure at (23 + 2)C and (50 + 5)% RH. The dish
contains a saturated solution of ammonium dihydrogen phosphate (NH4H2PO4).
The results are expressed in metres (of air) and the resistance to water vapour diffusion is
determined as mean value and round expediently to 1/10 m (one decimal).
188.8.131.52 Release of dangerous substances
Presence of dangerous substances in the product: The applicant shall submit a written
declaration stating whether or not the product/kit contains dangerous substances according to
European and national regulations, when and where relevant in the Member States of
destination, and shall list these substances.
Compliance with the applicable regulations:
If the product/kit contains dangerous substances as declared above, the ETA will provide the
method(s) which has been used for demonstrating compliance with the applicable regulations
in the Member States of destination, according to the dated EU data-base (method(s) of
content or release, as appropriate).
Application of the precautionary principle:
An EOTA member has the possibility to provide to the other members, through the Secretary
General, warning about substances which, according to Health authorities of its country, are
considered to be dangerous under sound scientific evidence, but are not yet regulated.
Complete references about this evidence will be provided.
This information once agreed upon, will be kept in an EOTA data base, and will be transferred
to the Commission services.
The information contained in this EOTA data base will also be communicated to any ETA
On the basis of this information, a protocol of assessment of the product, regarding this
substance, could be established on request of a manufacturer with the participation of the
Approval Body which raised the issue.
5.1.4 Safety in use
ETAG 004 42
Which ever type of fixing used, the bond strength between the base coat and the insulation
product shall be tested according to 184.108.40.206.1.
Furthermore, depending on the fixing type, the stability of the ETICS on the substrate should be
verified according to the tests specified in Table 3 and examination of the substrate as
described in chapter 7.
For mechanically fixed ETICS, the admissible load to be applied to an anchor is that stated in an
ETA or that determined according to the EOTA Guideline "Plastic anchors for fixing of external
thermal insulation composite systems with rendering (short form: Plastic anchors for ETICS).
Table 3: Tests for verifying the safety in use
Fully or partially Anchors fixed through the reinforcement
Anchors fixed through the insulation product
Bond strength between base coat and insulation product according to 220.127.116.11.1 Cellular plastic
(EN 13163 EN 13164 EN 13165 EN 13166)
Bond strength 18.104.22.168.2
Static foam block test 22.214.171.124.2
Pull-through test 126.96.36.199.1
Static foam block test 188.8.131.52.2
Static foam block test 184.108.40.206.2
Bond strength between base coat and insulation product according to 220.127.116.11.1
Bond strength 18.104.22.168.2
Dynamic wind uplift test
Dynamic wind uplift test 22.214.171.124.3
Dynamic wind uplift test 126.96.36.199.3
Dynamic wind uplift test 188.8.131.52.3
1) The tests on bonded ETICS with supplementary mechanical fixing devices should be
conducted without the fixings. 2)
The tests on mechanically fixed ETICS with supplementary adhesive should be conducted
without the adhesive. If the bonded area is less than 20 %, the ETICS is considered to be
purely mechanically fixed. 3)
Decision on which test to perform is based on Fig. 7. 4)
Only for ETICS not fulfilling the criteria in 184.108.40.206.
220.127.116.11 Bond strength
18.104.22.168.1 Bond strength between base coat and insulation product
ETAG 004 43
The following tests are performed:
on a panel of the insulation product faced with the base coat applied in accordance with
the ETA-applicants instructions and dried for at least 28 days under the same conditions
as the rig.
on samples taken from the rig after hygrothermal cycles (heat-rain and heat-cold cycles)
or on separated samples placed in the window of the rig (only if the low part of the rig
does not only consist of the reinforced base coat alone, i.e. ETICS with only one finishing
coat), test being always performed after at least 7 days drying.
if freeze-thaw cycles necessary according to 22.214.171.124:on the samples of reinforced base
coat alone after the freeze-thaw cycles as foreseen in 126.96.36.199.2 and dried for at least 7
days after the end of the cycles .
Five squares with appropriate sample size are cut through the base coat according to Fig. 4
using an angle grinder. The dimensions should be the same as the samples for testing the
tensile strength perpendicular to the faces according to the respective technical specification
of the insulation product (hEN or ETA acc. to ETAG or CUAP). Square metal plates of
appropriate size are affixed to these areas with a suitable adhesive.
The pull-off test (see Fig. 4) is performed at a tensioning speed of 1 to 10 mm/minute.
The mean failure resistance is based on the results of five tests.
The individual and mean values are recorded and the results are expressed in N/mm (MPa).
Fig. 4: Pull-off test
188.8.131.52.2 Bond strength test between adhesive and substrate
The test shall be carried out for bonded ETICS only.
The tests are performed on the following substrates:
- A substrate consisting of a smooth concrete slab at least 40 mm thick.
The water/cement ratio shall be of the order of 0.45 to 0.48. The tensile strength of the
slab shall be at least 1.5 N/mm. The moisture content of the slab prior to the test shall
be a maximum of 3 % of the total weight.
- For cement-free adhesive the most absorbent substrate of those specified by the
The adhesive is spread on the substrate to a thickness of 3 to 5 mm. After allowing the
adhesive to cure at (23 + 2)C and (50 + 5) % RH for at least 28 days, 15 squares 15 to 25
cm in area are cut through the adhesive according to Fig. 4. Metal plates of appropriate size
are bonded to it using a suitable adhesive.
ETAG 004 44
The pull-off test (see Fig. 4) is performed at a tensioning speed of 1 to 10 mm/minute on the
following samples (5 s